Chemical Composition of Wood
Table 1 presents major chemical compositions of some wood species. Each of these
components contributes to fiber properties, which ultimately impact product properties.
Cellulose (%) 40 39.5 45.0 41.0 Hemicellulose -Glucomannan (%) 16.0 17.2 3.1 2.3 -Glucuronoxylan (%) 8.9 10.4 14.1 27.5 -Other polysaccharides (%) 3.6 3.0 2.0 2.6 Lignin (%) 27.7 27.5 31.3 22.0 Total extractives (%) 3.5 2.1 2.8 3.0
HOH2C OH 1 HOH2C OH 1 O HO O HO O 4 O 4 O O 4 O 4 HO O HO O HOH C 1 OH 1 2 OH HOH2C
Figure 1. The Structure of Cellulose
Cellulose, the major chemical component of fiber wall and contributing 40-45% of the
wood’s dry weight, is composed of linear chains of D-glucose linked by ß-1,4-glycosidic bonds (Figure 2.1) with the degree of polymerization from 10,000 in native wood to 1,000 in bleached kraft pulps. Each D-anhydroglucopyranose unit possesses hydroxyl groups at C2,
C3, and C6 positions, capable of undergoing the typical reactions known for primary and
1 secondary alcohols. The molecular structure imparts cellulose with its characteristic
properties: hydrophylicity, chirality, degradability, and broad chemical variability initiated by the high donor reactivity of hydroxyl groups.
Cellulose has a strong tendency to form intra- and inter-molecular hydrogen bonds by the hydroxyl groups on these linear cellulose chains, which stiffen the straight chain and promote aggregation into a crystalline structure and give cellulose a multitude of partially crystalline fiber structures and morphologies.2 The degree of crystallinity of
different cellulose samples are presented in Table 2.3
Table 2. X-Ray Crystallinity of Some Cellulose Materials Sample X-ray crystallinity (%) Cotton linters 56-63 Sulfite dissolving pulp 50-56 Prehydrolyzed sulfate pulp 46 Viscose rayon 27-40 Regenerated cellulose film 40-45
The ultrastructure of native cellulose (cellulose I) has been discovered to possess
4 unexpected complexity in the form of two crystal phases: Iα and Ιβ. The relative amounts
Iα and Ιβ has been determined recently by Nishiyama et al using atomic-resolution
synchrotron and neutron diffraction data recorded from oriented fibrous samples prepared
2 by aligning cellulose microcrystals from the cell wall of the freshwater alga  and
The presence of crystalline cellulose, with regions of less order, and the size of the
elementary fibrils work together to produce interesting combination of contrary
properties such as stiffness and rigidity on one hand and flexibility on the other hand.7
Crystalline cellulose has a very limited accessibility to water and chemicals. Chemical attack can therefore be expected to occur primarily on amorphous cellulose and crystalline surface.
1 HOH 2C 1 HOH C RO 2 O O RO β O OR O 4 β O OR O 4 O 4 OR HO O RO O OH 14 1 HOH2C O 6
1 HO OH α
HOH2C O HO
4-β−D-Glcp-1 4-β−D-Manp-1 4-β−D-Manp-1 4-β−D-Manp-1 6 2,3
1 Ac α-D-Galp
Figure 2. Principal Structure of Galactoglucomannans in Softwood Sugar units: β-D-glucopyranose (GlcP); β-D-mannopyranose (Manp); β-D-galactopyranose (Galp). R = CH3CO or H. The lower representation is the abbreviated formula showing the proportions of the units (galactose-rich fraction)
Unlike cellulose, hemicelluloses have lower DP (only 50-300) with side groups on
the chain molecule and are essentially amorphous. The main hemicelluloses of softwood
are galactoglucomannans (Figure 2) and arabinoglucuronoxylan (Figure 3), while in
3 hardwood is glucuronoxylan (Figure 4). Table 2 summarizes the main structural features of hemicelluloses appearing in both softwood and hardwood.
1 1 OH 4 OH O OH O OH O 4 β O O O β O HO O O O 4 O 1 3 OH 1 4 O OH HO 1 1α α OH H3CO O HOOC HOH2C OH
4- D-Xylp-1 4-β−D-Xyp-1 4-β−D-Xylp-1 4-β−D-Xylp-1 4-β−D-Xylp-1 β− 2 3 5
1 1 4-O-Me-α−D-Glc pA α-L-Araf 2
Figure 3. Principal Structure of Arabinoglucuronoxylan in Softwood Sugar units: β-D-xylopyranose (XylP); 4-O-methyl-α-D-glucopyranosyluronic acid (GlcpA); α-L- Arobinofuranose (Araf). The lower representation is the abbreviated formula showing the proportions of the units.
4-β−D-Xylp-1 4-β−D-Xylp-1 4-β−D-Xylp-1 4-β−D-Xylp-1 2,3 2
R 1 7 4−Ο−Μ e−α−D-Glc pA
Figure 4. Principal Structure of Glucuronoxylan in Hardwood Sugar units: β-D-xylopyranose (XylP); 4-O-methyl-α-D-glucopyranosyluronic acid (GlcpA); R = Acetyl group (CH3CO).
4 Table 2. The Major Hemicellulose Components in Softwood and Hardwood1
Wood Hemicellulose Amount Composition DP type (% on wood) Units Molar Linkage ratios 3 SW Galacto- 5-8 β-D-Manp 1 → 4 100 glucomannan β-D-Glcp 1 1 → 4 α-D-Galp 1 1 → 6 Acetyl 1
(Galacto)- 10-15 β-D-Manp 4 1 → 4 100 glucomannan β-D-Glcp 1 1 → 4 α-D-Galp 0.1 1 → 6 Acetyl 1
Arabino- 7-10 β-D-Xylp 10 1 → 4 100 glucuronoxylan 4−Ο−Μe−α-D- 2 1 → 2 GlcpA 1 → 3 α-L-Araf 1.3
HW 10 Glucuronoxylan 15-30 β-D-Xylp 1 → 4 200 4−Ο−Μe−α-D- 1 1 → 2 GlcpA Acetyl 7
1-2 Glucomannan 2-5 β-D-Manp 1→ 4 200 β-D-Glcp 1 1→ 4
Figure 4) and has a molecular structure similar to cellulose when their branches are
removed from xylan, which may make xylan combine with cellulose in more ordered
structure after kraft pulping.8
Glucomannan is very sensitive to kraft cooking conditions and is already dissolved
to a large extent at the beginning of kraft cooking, whereas xylan is more resistant.7
Therefore, the content of xylan in chemical softwood kraft pulp becomes almost the same
5 as that of glucomannan in spite of considerably higher content of glucomannan in softwood (Table 3). Hemicelluloses in hardwood kraft pulps are dominated by xylan.
Furthermore, relocation of xylan in fiber can occur during kraft cooking due to the sorption of xylan from cooking liquor. Consequently, enhanced hemicellulose (xylan) levels on pulp fiber surfaces have been reported for both softwood and hardwood kraft pulps.9
Table 3. The Change of Chemical Composition of Birch and Pine Constituents Pine Birch (Pinus (Betula sylvestris) verrucosa) Cellulose (%) 40.0 41.0 Hemicellulose -Glucomannan (%) 16.0 2.3 -Glucuronoxylan (%) 8.9 27.5 -Other polysaccharides (%) 3.6 2.6 Lignin (%) 27.7 22.0 Total extractives (%) 3.5 3.0
In addition, all sugar components can take part in the formation of lignin carbohydrate complexes by covalent linkages between lignin and carbohydrates in both wood and pulps.10 The most frequently suggested LCC-linkages in native wood are benzyl ester, benzyl either, and glycosidic linkages. However, the benzyl ester linkage is alkali-labile and may therefore be hydrolyzed during kraft pulping process. The latter two linkages are alkali-stable and would survive from the hydrolysis during kraft pulping process.
6 Proximate Analysis of Wood
Typical Wood Properties
Wood Oven Calorif % % α % Pentosan % Extractives % Ash
Species Dry Value Lignin Cellulose
Western 35 .0 25.4 42.3 7.9 8.3 0.3
White 416 27.8 42.1 12.1 2.3
Black 400 27.3 45.8 12.5 2.2 0.29
Norway 368 26.9 42.3 11.0 0.9 0.31
Loblolly 545 4381 28.1 43.3 12.6 3.8 0.4
Slash Pine 560 4281 28.0 46.1 8.6 2.6 0.6
Jack Pine 4962 28.3 45.2 11.3 4.0 1.3
Wood Oven Calorif % % α % Pentosan % Extractives % Ash
Species Dry Value Lignin Cellulose
Yellow 657 3215 21.2 49.4 21.4 2.6 2.9 – 1.7
Red Maple 561 22.8 44.5 17.1 2.5 5.2
Yellow 432 4275 25.3 33.5 20.1 3.6 2.8
Quaking 400 3215 18.2 50.2 17.5 2.4 4
*kg/cu m; ** kcal/kg aid dry
1 Sjostrom, E., Wood Chemistry. Fundamentals and Applications. Second edition ed. 1993, San Diego: Academic press. 292.
2 Klemn, D., Heublein, B., Fink, H.-P., Bohn, A., Cellulose: Fascinating biopolymer and sustainable raw material. Angew. Chem. Int. Ed., 2005. 44: p. 3358-3393.
3 Klemn, D., Philipp, B., Heinze, T., Heinze, U., Wagenknecht, W., Comprehensive cellulose chemistry. Fundamentals and analytical methods. Vol. 1. 1998, Weinhein, Germany: WILEY-VCH. 266.
4 Atalla, R.H., VanderHart, D.L., Native cellulose: A composite of two distinct crystalline forms. Science, 1984. 223(4633): p. 283-285.
20(6): p. 1440-1442; Sugiyama, J., Persson, J., Chanzy, H., Combined infrared and electron diffraction study of the polymorphism of native celluloses. Macromolecules, 1991. 24(6): p. 2461-2469.
6 Nishiyama, Y., Sugiyama, J., Chanzy, H., Langan, P., Crystal structure and hydrogen bonding system in cellulose Iα from synchrotron X-ray and neutron fibrious diffraction. J. Am. Chem. Soc, 2003. 125: p. 14300-14306; Nishiyama, Y., Sugiyama, J., Chanzy, H., Langan, P., Crystal structure and hydrogen bonding system in cellulose Iβ from synchrotron X-ray and neutron fibrious diffraction. J. Am. Chem. Soc, 2002. 124: p. 9074-9082.
7 Wagberg, L., Annergren, G.O. Physicochemical characterization of papermaking fibers, in: The fundamentals of Papermaking Materials: Transaction of the 11th Fundamental Research Symposium in Held at Cambridge, C.F. Baker, Editor. 1997, Pira International. p. 1-82.
8 Mitikka, M., Teeaar, R., Tenkanene, M., Laine, J., Vuorinene, T., Sorption of xylans on cellulose fibers, in 8th International Symposium on Wood and Pulping Chemistry. 1995: Helsinki, Finland. p. 231-236.
9 Kibblewhite, R.P., Brookes, D., Distribution of chemical compositions in the walls of kraft and bisulfite pulp fibers. Wood Sci. Technol., 1976. 10(1): p. 39-46; Suurnakki, A., Westermak, U., Chemical characterization of the surface layers of unbleached Pine [Pinus] and Birch [Betula] kraft pulp fibers. J. Pulp Pap. Sci., 1996. 22(2): p. J43-J47.
10 Erilkssen, O., Goring, D.A.I., Lindgren, B.O., Structural studies on chemical bonds between lignins and carbohydrates in spruce wood. Wood Sci. Technol., 1980. 14: p. 267-279; Iversen, T., Lignin-carbohydrate bonds in lignin-carbohydrate complex isolated from spruce. Wood Sci. Technol., 1985. 19: p. 243-251; Iversen, T., Westermark, U., Lingnin-carbohydrate bonds n pine lignins dissolved during kraft pulping. Cellulose Chem. Technol., 1985. 19: p. 531-536; Iversen, T., Wannstrom, S., Lignin-carbohydrate bonds in residual lignin isolated from pine kraft pulp. Holzforschung, 1986. 40: p. 19-22; Iversen, T., Westermark, U., Samuelsson, B., Some components on the isolation of galactose-containing lignin-carbohydrate complexes. Holzforschung, 1987. 41: p. 119- 121.